LMucko/crystallography-open-database huggingface dataset:
On the crystallographic and magnetic structures of nearly stoichiometric iron monoxide Sample: T = 298 K
Fjellvag, H.; Gronvold, F.; Stolen, S.; Hauback, B. C.; Journal of Solid State Chemistry 124 (1996) 52–57; doi:10.1006/jssc.1996.0206

data_9009768
_publ_section_title
;
 On the crystallographic and magnetic structures of
 nearly stoichiometric iron monoxide
 Sample: T = 298 K
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              52
_journal_page_last               57
_journal_paper_doi               10.1006/jssc.1996.0206
_journal_volume                  124
_journal_year                    1996
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe3 O4'
_chemical_name_mineral           Magnetite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.4045
_cell_length_b                   8.4045
_cell_length_c                   8.4045
_cell_formula_units_Z            8
_cell_volume                     593.657
_database_code_amcsd             0013895
_diffrn_ambient_temperature      298
_exptl_crystal_density_diffrn    5.181
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_database_code               9009768
On the crystallographic and magnetic structures of nearly stoichiometric iron monoxide Sample: T = 12 K
Fjellvag, H.; Gronvold, F.; Stolen, S.; Hauback, B. C.; Journal of Solid State Chemistry 124 (1996) 52–57; doi:10.1006/jssc.1996.0206

data_9009769
_publ_section_title
;
 On the crystallographic and magnetic structures of
 nearly stoichiometric iron monoxide
 Sample: T = 12 K
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              52
_journal_page_last               57
_journal_paper_doi               10.1006/jssc.1996.0206
_journal_volume                  124
_journal_year                    1996
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe3 O4'
_chemical_name_mineral           Magnetite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3873
_cell_length_b                   8.3873
_cell_length_c                   8.3873
_cell_formula_units_Z            8
_cell_volume                     590.020
_database_code_amcsd             0013896
_diffrn_ambient_temperature      12
_exptl_crystal_density_diffrn    5.213
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_database_code               9009769
On the crystallographic and magnetic structures of nearly stoichiometric iron monoxide Note: low-temperature polymorph Sample: Three-Phase Mixture FeO, T = 12 K
Fjellvag, H.; Gronvold, F.; Stolen, S.; Hauback, B. C.; Journal of Solid State Chemistry 124 (1996) 52–57; doi:10.1006/jssc.1996.0206

data_9009770
_publ_section_title
;
 On the crystallographic and magnetic structures of
 nearly stoichiometric iron monoxide
 Note: low-temperature polymorph
 Sample: Three-Phase Mixture FeO, T = 12 K
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              52
_journal_page_last               57
_journal_paper_doi               10.1006/jssc.1996.0206
_journal_volume                  124
_journal_year                    1996
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe O'
_chemical_name_mineral           Wuestite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-P 3*'
_symmetry_space_group_name_H-M   'R -3 :R'
_cell_angle_alpha                59.34
_cell_angle_beta                 59.34
_cell_angle_gamma                59.34
_cell_length_a                   6.132
_cell_length_b                   6.132
_cell_length_c                   6.132
_cell_formula_units_Z            8
_cell_volume                     160.589
_database_code_amcsd             0013897
_diffrn_ambient_temperature      12
_exptl_crystal_density_diffrn    5.943
_cod_original_sg_symbol_H-M      'R -3'
_cod_database_code               9009770
On the crystallographic and magnetic structures of nearly stoichiometric iron monoxide Note: low-temperature polymorph Sample: Single-Phase Fe0.925O, T = 12 K
Fjellvag, H.; Gronvold, F.; Stolen, S.; Hauback, B. C.; Journal of Solid State Chemistry 124 (1996) 52–57; doi:10.1006/jssc.1996.0206

data_9009771
_publ_section_title
;
 On the crystallographic and magnetic structures of
 nearly stoichiometric iron monoxide
 Note: low-temperature polymorph
 Sample: Single-Phase Fe0.925O, T = 12 K
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              52
_journal_page_last               57
_journal_paper_doi               10.1006/jssc.1996.0206
_journal_volume                  124
_journal_year                    1996
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.925 O'
_chemical_name_mineral           Wuestite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-P 3*'
_symmetry_space_group_name_H-M   'R -3 :R'
_cell_angle_alpha                59.92
_cell_angle_beta                 59.92
_cell_angle_gamma                59.92
_cell_length_a                   6.073
_cell_length_b                   6.073
_cell_length_c                   6.073
_cell_formula_units_Z            8
_cell_volume                     158.091
_database_code_amcsd             0013898
_diffrn_ambient_temperature      12
_exptl_crystal_density_diffrn    5.685
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        'Fe.925 O'
_cod_database_code               9009771
Analysis and structural determination of Nd-substituted zirconolite-4M
Coelho, A. A.; Cheary, R. W.; Smith, K. L.; Journal of Solid State Chemistry 129 (1997) 346–359; doi:10.1006/jssc.1996.7263

data_9009772
_publ_section_title
;
 Analysis and structural determination of Nd-substituted zirconolite-4M
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              346
_journal_page_last               359
_journal_paper_doi               10.1006/jssc.1996.7263
_journal_volume                  129
_journal_year                    1997
_chemical_compound_source        Synthetic
_chemical_formula_structural     Ca.721Nd.494Zr.772Ti1.997O7
_chemical_formula_sum            'Ca2.55 Nd1.91 O28 Ti7.28 Zr3.22'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 84.791
_cell_angle_gamma                90
_cell_length_a                   12.522
_cell_length_b                   7.222
_cell_length_c                   22.987
_cell_formula_units_Z            4
_cell_volume                     2070.219
_database_code_amcsd             0013921
_exptl_crystal_density_diffrn    4.710
_cod_original_formula_sum        'Ca2.55 Nd1.91 Zr3.22 Ti7.28 O28'
_cod_database_code               9009772
_amcsd_formula_title             Ca.721Nd.494Zr.772Ti1.997O7
Hydrogen bonding and Jahn-Teller distortion in groutite, alpha-MnOOH, and manganite, gamma-MnOOH, and their relations to the manganese dioxides ramsdellite and pyrolusite
Kohler, T.; Armbruster, T.; Libowitzky, E.; Journal of Solid State Chemistry 133 (1997) 486–500; doi:10.1006/jssc.1997.7516

data_9009773
_publ_section_title
;
 Hydrogen bonding and Jahn-Teller distortion in groutite, alpha-MnOOH,
 and manganite, gamma-MnOOH, and their relations to the manganese
 dioxides ramsdellite and pyrolusite
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              486
_journal_page_last               500
_journal_paper_doi               10.1006/jssc.1997.7516
_journal_volume                  133
_journal_year                    1997
_chemical_compound_source
'Nchwaning Mine, Kalahari manganese field, Republic of South Africa'
_chemical_formula_sum            'H Mn O2'
_chemical_name_mineral           Groutite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.667
_cell_length_b                   2.871
_cell_length_c                   4.554
_cell_formula_units_Z            4
_cell_volume                     139.466
_database_code_amcsd             0013941
_exptl_crystal_density_diffrn    4.188
_cod_original_formula_sum        'Mn O2 H'
_cod_database_code               9009773
Hydrogen bonding and Jahn-Teller distortion in groutite, alpha-MnOOH, and manganite, gamma-MnOOH, and their relations to the manganese dioxides ramsdellite and pyrolusite Note: Uiso corrected
Kohler, T.; Armbruster, T.; Libowitzky, E.; Journal of Solid State Chemistry 133 (1997) 486–500; doi:10.1006/jssc.1997.7516

data_9009774
_publ_section_title
;
 Hydrogen bonding and Jahn-Teller distortion in groutite, alpha-MnOOH,
 and manganite, gamma-MnOOH, and their relations to the manganese
 dioxides ramsdellite and pyrolusite
 Note: Uiso corrected
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              486
_journal_page_last               500
_journal_paper_doi               10.1006/jssc.1997.7516
_journal_volume                  133
_journal_year                    1997
_chemical_compound_source
'Nchwaning Mine, Kalahari manganese field, Republic of South Africa'
_chemical_formula_sum            'H Mn O2'
_chemical_name_mineral           Manganite
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 114.38
_cell_angle_gamma                90
_cell_length_a                   5.304
_cell_length_b                   5.277
_cell_length_c                   5.304
_cell_formula_units_Z            4
_cell_volume                     135.217
_database_code_amcsd             0013942
_exptl_crystal_density_diffrn    4.320
_cod_original_formula_sum        'Mn O2 H'
_cod_database_code               9009774
Characterization of ternary compounds in the BaO:Fe2O3:TiO2 system: Ba6Fe45Ti17O106 and BaFe11Ti3O23 Note: data from neutron and synchrotron radiation on powder
Vanderah, T. A.; Wong-Ng W; Toby, B. H.; Browning, V. M.; Shull, R. D.; Geyer, R. G.; Roth, R. S.; Journal of Solid State Chemistry 143 (1999) 182–197; doi:10.1006/jssc.1999.8075

data_9009775
_publ_section_title
;
 Characterization of ternary compounds in the BaO:Fe2O3:TiO2
 system: Ba6Fe45Ti17O106 and BaFe11Ti3O23
 Note: data from neutron and synchrotron radiation on powder
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              182
_journal_page_last               197
_journal_paper_doi               10.1006/jssc.1999.8075
_journal_volume                  143
_journal_year                    1999
_chemical_formula_structural     Ba6Fe45Ti17O106
_chemical_formula_sum            'Ba3 Fe21.85 O53 Ti9.15'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.2734
_cell_angle_gamma                90
_cell_length_a                   19.4119
_cell_length_b                   20.2777
_cell_length_c                   10.0831
_cell_formula_units_Z            4
_cell_volume                     3828.812
_exptl_crystal_density_diffrn    5.063
_cod_original_formula_sum        'Ba3 Fe21.85 Ti9.15 O53'
_cod_database_code               9009775
Characterization of ternary compounds in the BaO:Fe2O3:TiO2 system: Ba6Fe45Ti17O106 and BaFe11Ti3O23 Note: data from single-crystal X-ray diffraction
Vanderah, T. A.; Wong-Ng W; Toby, B. H.; Browning, V. M.; Shull, R. D.; Geyer, R. G.; Roth, R. S.; Journal of Solid State Chemistry 143 (1999) 182–197; doi:10.1006/jssc.1999.8075

data_9009776
_publ_section_title
;
 Characterization of ternary compounds in the BaO:Fe2O3:TiO2
 system: Ba6Fe45Ti17O106 and BaFe11Ti3O23
 Note: data from single-crystal X-ray diffraction
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              182
_journal_page_last               197
_journal_paper_doi               10.1006/jssc.1999.8075
_journal_volume                  143
_journal_year                    1999
_chemical_formula_structural     BaFe11Ti3O23
_chemical_formula_sum            'Ba Fe11.04 O23 Ti2.96'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.62
_cell_angle_gamma                90
_cell_length_a                   19.561
_cell_length_b                   8.6614
_cell_length_c                   10.120
_cell_formula_units_Z            4
_cell_volume                     1651.265
_database_code_amcsd             0013968
_exptl_crystal_density_diffrn    5.083
_cod_original_formula_sum        'Ba Fe11.04 Ti2.96 O23'
_cod_database_code               9009776
_amcsd_formula_title             BaFe11Ti3O23
The crystal structures of the binary valence compound Bi3BiO7 and isotypic Bi3SbO7 as determined by high resolution X-ray and neutron powder diffraction
Dinnebier, R. E.; Ibberson, R. M.; Ehrenberg, H.; Jansen, M.; Journal of Solid State Chemistry 163 (2002) 332–339; doi:10.1006/jssc.2001.9427

data_9009777
_publ_section_title
;The crystal structures of the binary valence compound Bi3BiO7 and isotypic
 Bi3SbO7 as determined by high resolution X-ray and neutron powder diffraction
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              332
_journal_page_last               339
_journal_paper_doi               10.1006/jssc.2001.9427
_journal_volume                  163
_journal_year                    2002
_chemical_formula_structural     Bi4O7
_chemical_formula_sum            'Bi4 O7'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                72.566
_cell_angle_beta                 88.842
_cell_angle_gamma                76.925
_cell_length_a                   6.7253
_cell_length_b                   6.9950
_cell_length_c                   7.7961
_cell_formula_units_Z            2
_cell_volume                     340.390
_database_code_amcsd             0014020
_exptl_crystal_density_diffrn    9.249
_cod_database_code               9009777
_amcsd_formula_title             Bi4O7
The crystal structures of the binary valence compound Bi3BiO7 and isotypic Bi3SbO7 as determined by high resolution X-ray and neutron powder diffraction
Dinnebier, R. E.; Ibberson, R. M.; Ehrenberg, H.; Jansen, M.; Journal of Solid State Chemistry 163 (2002) 332–339; doi:10.1006/jssc.2001.9427

data_9009778
_publ_section_title
;The crystal structures of the binary valence compound Bi3BiO7 and isotypic
 Bi3SbO7 as determined by high resolution X-ray and neutron powder diffraction
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              332
_journal_page_last               339
_journal_paper_doi               10.1006/jssc.2001.9427
_journal_volume                  163
_journal_year                    2002
_chemical_formula_structural     Bi3SbO7
_chemical_formula_sum            'Bi3 O7 Sb'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                73.388
_cell_angle_beta                 89.225
_cell_angle_gamma                76.190
_cell_length_a                   6.6044
_cell_length_b                   7.0146
_cell_length_c                   7.6048
_cell_formula_units_Z            2
_cell_volume                     327.278
_database_code_amcsd             0014021
_exptl_crystal_density_diffrn    8.734
_cod_original_formula_sum        'Bi3 Sb O7'
_cod_database_code               9009778
_amcsd_formula_title             Bi3SbO7
Structural relations between weberite and zirconolite polytypes - refinements of doped 3T and 4M Ca2Ta2O7 and 3T CaZrTi2O7 Locality: synthetic Sample: T = 123 K Note: polytype Zirconolite-3T
Grey, I. E.; Mumme, W. G.; Ness, T. J.; Roth, R. S.; Smith, K. L.; Journal of Solid State Chemistry 174 (2003) 285–295; doi:10.1016/S0022-4596(03)00222-6

data_9009779
_publ_section_title
;Structural relations between weberite and zirconolite polytypes - refinements
 of doped 3T and 4M Ca2Ta2O7 and 3T CaZrTi2O7 Locality: synthetic Sample: T =
 123 K Note: polytype Zirconolite-3T
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              285
_journal_page_last               295
_journal_paper_doi               10.1016/S0022-4596(03)00222-6
_journal_volume                  174
_journal_year                    2003
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.96 Ca1.538 O14 Th0.302 Ti2.6 Zr2.6'
_chemical_name_mineral           Zirconolite
_space_group_IT_number           152
_symmetry_space_group_name_Hall  'P 31 2"'
_symmetry_space_group_name_H-M   'P 31 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   7.228
_cell_length_b                   7.228
_cell_length_c                   16.805
_cell_formula_units_Z            3
_cell_volume                     760.336
_database_code_amcsd             0014037
_diffrn_ambient_temperature      123
_exptl_crystal_density_diffrn    4.870
_cod_original_formula_sum        'Ca1.538 Th.302 Zr2.6 Ti2.6 Al.96 O14'
_cod_database_code               9009779
The crystal structures of the cubic forms of arsenious and antimonous oxides Note: synthetic sample
Bozorth, R. M.; Journal of the American Chemical Society 45 (1923) 1621–1627; doi:10.1021/ja01660a006

data_9009780
_publ_section_title
;
 The crystal structures of the cubic forms of arsenious and antimonous oxides
 Note: synthetic sample
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              1621
_journal_page_last               1627
_journal_paper_doi               10.1021/ja01660a006
_journal_volume                  45
_journal_year                    1923
_chemical_formula_sum            'As2 O3'
_chemical_name_mineral           Arsenolite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   11.06
_cell_length_b                   11.06
_cell_length_c                   11.06
_cell_formula_units_Z            16
_cell_volume                     1352.899
_exptl_crystal_density_diffrn    3.885
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_database_code               9009780
_cod_duplicate_entry 1010609
The crystal structures of the cubic forms of arsenious and antimonous oxides Locality: Mt. Hamimat, Algeria
Bozorth, R. M.; Journal of the American Chemical Society 45 (1923) 1621–1627; doi:10.1021/ja01660a006

data_9009781
_publ_section_title
;
 The crystal structures of the cubic forms of arsenious and antimonous oxides
 Locality: Mt. Hamimat, Algeria
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              1621
_journal_page_last               1627
_journal_paper_doi               10.1021/ja01660a006
_journal_volume                  45
_journal_year                    1923
_chemical_formula_sum            'O3 Sb2'
_chemical_name_mineral           Senarmontite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   11.14
_cell_length_b                   11.14
_cell_length_c                   11.14
_cell_formula_units_Z            16
_cell_volume                     1382.470
_exptl_crystal_density_diffrn    5.602
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Sb2 O3'
_cod_database_code               9009781
_cod_duplicate_entry 1011218
Crystal structures of hematite and corundum
Pauling, L.; Hendricks, S. B.; Journal of the American Chemical Society 47 (1925) 781–790; doi:10.1021/ja01680a027

data_9009782
_publ_section_title
;
 Crystal structures of hematite and corundum
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              781
_journal_page_last               790
_journal_paper_doi               10.1021/ja01680a027
_journal_volume                  47
_journal_year                    1925
_chemical_formula_sum            'Fe2 O3'
_chemical_name_mineral           Hematite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-P 3* 2n'
_symmetry_space_group_name_H-M   'R -3 c :R'
_cell_angle_alpha                55.28
_cell_angle_beta                 55.28
_cell_angle_gamma                55.28
_cell_length_a                   5.420
_cell_length_b                   5.420
_cell_length_c                   5.420
_cell_formula_units_Z            2
_cell_volume                     100.236
_database_code_amcsd             0014076
_exptl_crystal_density_diffrn    5.291
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_database_code               9009782
Crystal structures of hematite and corundum Locality: Ceylon
Pauling, L.; Hendricks, S. B.; Journal of the American Chemical Society 47 (1925) 781–790; doi:10.1021/ja01680a027

data_9009783
_publ_section_title
;
 Crystal structures of hematite and corundum
 Locality: Ceylon
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              781
_journal_page_last               790
_journal_paper_doi               10.1021/ja01680a027
_journal_volume                  47
_journal_year                    1925
_chemical_formula_sum            'Al2 O3'
_chemical_name_mineral           Corundum
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-P 3* 2n'
_symmetry_space_group_name_H-M   'R -3 c :R'
_cell_angle_alpha                55.28
_cell_angle_beta                 55.28
_cell_angle_gamma                55.28
_cell_length_a                   5.120
_cell_length_b                   5.120
_cell_length_c                   5.120
_cell_formula_units_Z            2
_cell_volume                     84.496
_exptl_crystal_density_diffrn    4.008
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_database_code               9009783
_cod_duplicate_entry 1010914
Structure refinement of cubic As2O3 (arsenolithe) with single crystal data
Pertlik, F.; Czechoslovak Journal of Physics B 28 (1978) 170–176; doi:10.1007/BF01591036

data_9009784
_publ_section_title
;
 Structure refinement of cubic As2O3 (arsenolithe) with single crystal data
;
_journal_name_full               'Czechoslovak Journal of Physics B'
_journal_page_first              170
_journal_page_last               176
_journal_paper_doi               10.1007/BF01591036
_journal_volume                  28
_journal_year                    1978
_chemical_formula_sum            'As2 O3'
_chemical_name_mineral           Arsenolite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   11.074
_cell_length_b                   11.074
_cell_length_c                   11.074
_cell_formula_units_Z            16
_cell_volume                     1358.043
_database_code_amcsd             0012423
_exptl_crystal_density_diffrn    3.871
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_database_code               9009784